FORCE SPACE STUDIES OF ELASTOMERIC ANISOTROPICFIBRILLAR ADHESIVESA DISSERTATIONSUBMITTED TO THE DEPARTMENT OF APPLIED PHYSICSAND THE COMMITTEE ON GRADUATE STUDIESOF STANFORD UNIVERSITYIN PARTIAL FULFILLMENT OF THE REQUIREMENTSFOR THE DEGREE OFDOCTOR OF PHILOSOPHYDaniel Ruben SotoAugust 2010
6 Modeling 696.1 Peel Zone Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 696.2 Elastica Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 706.2.1 Cantilever with Point Load at End . . . . . . . . . . . . . . . 736.2.2 Fixed Slope at End of Beam . . . . . . . . . . . . . . . . . . . 776.3 Numerical Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 776.3.1 Validation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 776.3.2 Limit Surface Simulation . . . . . . . . . . . . . . . . . . . . . 827 Conclusion 897.1 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 897.2 Future Work . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 90A Beam Compliance Characterization 91A.1 Compliance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 91A.1.1 Axial Compliance . . . . . . . . . . . . . . . . . . . . . . . . . 91A.1.2 Lateral Compliance . . . . . . . . . . . . . . . . . . . . . . . . 93Bibliography 95ix
List of Tables5.1 Dual-axis cantilever stiffnesses . . . . . . . . . . . . . . . . . . . . . . 495.2 Comparison between measured and predicted array forces . . . . . . . 60x
List of Figures2.1 Idealized surface roughness . . . . . . . . . . . . . . . . . . . . . . . . 42.2 Idealized pressure sensitive adhesive . . . . . . . . . . . . . . . . . . . 52.3 Idealized fibrillar adhesive . . . . . . . . . . . . . . . . . . . . . . . . 62.4 Coulomb friction limit curve . . . . . . . . . . . . . . . . . . . . . . . 92.5 Coulomb friction limit curves . . . . . . . . . . . . . . . . . . . . . . 102.6 Embedded cone limit curve . . . . . . . . . . . . . . . . . . . . . . . . 112.7 Embedded cone limit curves . . . . . . . . . . . . . . . . . . . . . . . 122.8 Frictional adhesion limit surface . . . . . . . . . . . . . . . . . . . . . 153.1 Adhesive fabrication sequence . . . . . . . . . . . . . . . . . . . . . . 203.2 SU-8 mold on quartz wafer . . . . . . . . . . . . . . . . . . . . . . . . 233.3 Cast adhesive pillar array . . . . . . . . . . . . . . . . . . . . . . . . 243.4 Adhesive pillar array . . . . . . . . . . . . . . . . . . . . . . . . . . . 253.5 Adhesive pillar profile . . . . . . . . . . . . . . . . . . . . . . . . . . . 263.6 Adhesive mold overhang . . . . . . . . . . . . . . . . . . . . . . . . . 283.7 Adhesive pillar base detail . . . . . . . . . . . . . . . . . . . . . . . . 293.8 Incomplete mold etching . . . . . . . . . . . . . . . . . . . . . . . . . 303.9 Roughened pillar tip . . . . . . . . . . . . . . . . . . . . . . . . . . . 313.10 Escaped SU-8 bubbles . . . . . . . . . . . . . . . . . . . . . . . . . . 333.11 Escaped SU-8 bubble detail . . . . . . . . . . . . . . . . . . . . . . . 344.1 Limit surface test diagram . . . . . . . . . . . . . . . . . . . . . . . . 364.2 Limit surface test apparatus . . . . . . . . . . . . . . . . . . . . . . . 384.3 Force measurement system block diagram . . . . . . . . . . . . . . . 39xi
6.11 Limit curve simulation using elastica model. . . . . . . . . . . . . . . 876.12 Single adhesive pillar deflection . . . . . . . . . . . . . . . . . . . . . 88A.1 Axial compliance of adhesive pillar . . . . . . . . . . . . . . . . . . . 92A.2 Shear compliance of adhesive pillar . . . . . . . . . . . . . . . . . . . 94xiii
Chapter 1IntroductionThe elucidation of the structure of the gecko adhesive mechanism has revealed a newadhesive architecture and technology. Before the mechanisms of the gecko’s adhesivesystem were investigated, most known adhesive systems consisted of a very soft materialthat could create large surface areas between two rigid surfaces. Examples ofthis architecture include adhesive tape and the toes of many frogs. In each case atacky intermediate material is used to increase surface area. Conventional adhesivematerials are soft, with bulk moduli below 100 kPa . The gecko uses micron andnanometer scale hairs of β-keratin, which has a bulk modulus of 1.6 GPa , to formits adhesive. The material these hairs are made from is much stiffer than conventionaladhesive materials found on adhesive tape. This opens an avenue for the creation ofadhesives that no longer rely on the intrinsic properties of the adhesive material butrather on the geometry of the material. Conventional pressure sensitive adhesivematerials are subject to creep, outgassing, and temperature dependence. Adhesivesmade from suitably chosen materials can avoid these problems. Polydimethylsiloxane(PDMS rubber), polypropylene, and carbon nanotubes have been used to fabricategecko-inspired adhesives. These materials can be used for adhesives appropriate forhigh temperature or low pressure environments where traditional adhesive materialsare likely to fail.1
CHAPTER 1. INTRODUCTION 21.1 OutlineThis work describes the fabrication and investigation of a gecko-inspired artificialadhesive. In Chapter 2, useful background material is presented for understandingthis fibrillar artificial adhesive. This material includes models of adhesive behaviorand a review of previous fibrillar adhesives. The design and fabrication process ofthese adhesives is described in Chapter 3. In Chapter 4, fabricated arrays are testedand their adhesive properties are described. Individual adhesive elements are isolatedfrom arrays and tested in Chapter 5. In Chapter 6, models and simulations aredescribed that suggest that pillar shape plays a role in the type of adhesion observedand predict some of the behavior observed in the testing in Chapters 4 and 5.
Chapter 2BackgroundThis chapter provides a brief introduction to the theory of adhesives. This introductionprovides a basis of understanding for fibrillar adhesives and how they differ fromthe most familiar example, adhesive tape. The chapter ends with a review of othergecko inspired adhesives.2.1 Adhesion FundamentalsTo better understand fibrillar adhesives, it is useful to start with a discussion ofadhesion in general and the fundamentals of more familiar adhesives such as tape.Adhesives rely on intermolecular forces as the attractive forces between objects .2.1.1 van der Waals AdhesionChief among these intermolecular forces that are responsible for adhesion are thevan der Waals forces . These forces result from dipole moments in the materialsattracting each other. Even materials without permanent dipole moments such as noblegases, have instantaneous dipole moments from quantum-mechanical fluctuations.These fluctuating dipole moments result in an overall attractive force .At distances greater than several nanometers, these van der Waals forces fall offquickly and the maximum attractive force is found at a distance of a few nanometers.3
CHAPTER 2. BACKGROUND 4Figure 2.1: Depiction of surface roughness between two surfaces that are intendedto be adhered together. The top gray surface is depicted as perfectly smooth forsimplicity. The bottom blue surface shows a surface roughness common to mostmaterials. It is only in the regions around where contact is made that van der Waalsforces can act. In this case, this the area is very small.In order for this van der Waals attraction to create adhesive forces large enough tohold two objects in contact, the amount of area in close proximity must be large. Sincemost surfaces have a surface roughness that exceeds this nanometer length scale forattractive force, the surfaces must deform in order for large areas to be sufficientlyclose for the van der Waals interaction. In Figure 2.1 there is an idealized depictionof a perfectly smooth surface in contact with a rough surface. This image shows howvery close contact only occurs in a few locations while other areas are too far away forsignificant attractive force. In Figure 2.2 the yellow layer represents an intermediatelayer of adhesive between the smooth and rough surfaces. This adhesive layer is verysoft and able to deform so that large areas are in close contact with the rough surface.Pressure sensitive and fibrillar adhesives use two different approaches to create theselarge areas of intimate contact necessary for macroscopic adhesion.
CHAPTER 2. BACKGROUND 5Figure 2.2: Depiction of the role that a pressure sensitive adhesive (yellow) plays inincreasing the amount of intimate surface contact between two surfaces. In Figure2.1, only small areas were close enough for van der Waals interaction. The additionof the yellow intermediate material increases this intimate contact area.2.1.2 Pressure Sensitive AdhesivesPressure sensitive adhesives use a material that is very soft to create the intermediatelayer between two rigid materials. In addition to being soft, the material must alsobe cohesive enough to withstand tensile stress in the material. To see how a softcohesive material can create adhesion, we consider the amount of contact betweentwo surfaces having a pressure sensitive intermediary layer. The equilibrium area ofcontact can be thought of as the area that minimizes the following energy equationU total = −∆γA + U deformation (E, A) (2.1)where the first term (−∆γA) is the lowering of the energy of the system whenthe two surfaces make contact, and the second (U deformation (E, A)) the raising of thesystem’s energy as the material is deformed to cause a contact area A. The surfaceenergy per unit area ∆γ is a function of the material properties such as the polarizabilityand is directly proportional to the amount of area in contact. The deformation
CHAPTER 2. BACKGROUND 6Figure 2.3: Depiction of the role that a fibrillar adhesive (yellow) plays in increasingthe amount of intimate surface contact between two surfaces. In this case, the surfaceroughness is filled by fine hairs that can make contact at different distances from thesmooth surface. These hairs allow for more van der Waals interaction area comparedto the bare surfaces.energy is an increasing function of the amount of area in contact and the Young’sModulus or rigidity of the material.Carl Dahlquist determined empirically that a material with a Young’s Modulusless than 100 kPa is tacky . This means that the equilibrium value of A in Equation2.1 is large enough for the materials to exhibit adhesion.2.1.3 Fibrillar AdhesivesFibrillar adhesives do not rely on the low Young’s Modulus of an adhesive material.The gecko uses a material (β-keratin) that has a modulus of ∼2 GPa, roughly fourorders of magnitude above the Dahlquist criterion. The gecko makes this materialbehave like an adhesive by creating very fine, slender structures. These fine structurescreate a material that has an effective modulus that fulfills the Dahlquist criterion.The use of hairs rather than a planar layer allows the gecko adhesive to demonstrate
CHAPTER 2. BACKGROUND 7properties not seen in pressure-sensitive adhesives like tape or rubber cement.The most striking of the properties of the gecko adhesive that are a result ofits fibrillar structure is the directional or anisotropic behavior. This means thatdepending on the orientation of the gecko hairs and the direction of the stress applied,that the adhesive behavior will be different. The other property, though more subtle,is that the adhesion displayed by the gecko adhesive is qualitatively different thanthe type of adhesion displayed by pressure sensitive adhesives. We can visualize theseunique properties with the aid of a concept called the limit surface.2.2 Limit SurfaceTo understand the properties of these different adhesives, it is useful to look at theadhesive stresses in a space where the forces in x, y, and z directions are the axesof the space. We will call this space the force space. The limit surface is thenthe locus of points in this force space where relative movement between the twosurfaces occurs. This limit surface generally divides the force space into regionswhere stable attachment is possible and where relative movement of the adhesive andsubstrate (adhesive failure) will occur. For a limit surface, a sliding failure wherethe two surfaces are still in contact and a detachment failure where the two surfacesseparate are considered equivalent. Most of this discussion involves two-dimensionalforce spaces so, strictly speaking, we will be mainly discussing limit curves. Wecan empirically determine the limit curve of an adhesive contact by subjecting theadhesive interface to stress until the interface fails. To trace out the limit surface,these stresses should be in proportions varying between primarily normal stress andprimarily shear stress.2.2.1 Coulomb Friction Limit SurfaceA familiar system that we can use as a limit surface example is the ideal friction ofa block on an inclined plane. As we see in Figure 2.4, this limit surface is a simple
CHAPTER 2. BACKGROUND 8pair of sloped lines given byF N = 1 µ |F S|.For values of θ less than the critical angle θ c , the normal and shear forces at theinterface lie in the shaded region of the plot and the block does not slide. When theangle exceeds θ c , the force pair lies outside the stable grey region, the interface fails,and the block begins to slide. The shaded surface does not include any region withnegative values of F N which means that this interface cannot support any adhesion.We can envision other limit surfaces related to this ideal coulomb-friction surfaceto help build some intuition. First, consider a hockey puck or curling block on ice.The interface between the puck and the ice can be sheared with very little force.Assuming the surface obeys coulomb friction, the limit surface will be a v-shapedsurface with a relatively steep slope. The slope is equal to the reciprocal of thecoefficient of friction, so for ice, this slope will be of large magnitude. A smooth-soledshoe will also have a low-coefficient of friction on this smooth ice. This means thatattempting to create a large shear stress at the interface will lead to interface failure orslipping, a result familiar to anyone who has walked and fallen on ice. In contrast tothis situation, consider instead, rubber soled tennis shoes on asphalt. This interfacewill support a large amount of stress for a given normal force. This surface will havea lower magnitude slope and will include a greater percentage of the half of the forcespace that is compressive. We can take this limit surface to an extreme by imagininga frictionless, weightless, rigid dowel in a matching hole. In the normal direction,the dowel can be removed with any non-zero tensile force and can withstand anycompressive force. It can also bear any shear load without moving. In this case,the limit surface is the shear force axis and the stable region is the compressive halfspace.Each of these examples will demonstrate isotropic friction, that is, though weare considering limit curves in two dimensions, if we extend to three dimensions offorce space, these v-shaped curves will become cone-shaped surfaces. We now describesome anisotropic surfaces.If we consider the interaction of a skateboard and a concrete surface, we have ananisotropic limit surface. For forces along the long axis of the skateboard, there is very
CHAPTER 2. BACKGROUND 9stableunstableFigure 2.4: Coulomb friction limit curve. The gray area indicates pairs of normal andshear forces at the adhesive interface that remain attached. Pairs of forces below thered limit curve will result in the breaking of the adhesive interface. For a block ona plane, the force pairs form a circular arc with radius mg that sweeps a circle as θis increased. When θ is greater than the critical angle θ cr , the arc crosses the limitcurve and sliding begins. Also, if any tensile normal stress is created at the interfacethe surfaces will detach.
CHAPTER 2. BACKGROUND 10Zero FrictionLow FrictionHigh FrictionInfinite FrictionFigure 2.5: These four limit curves depict ideal Coulomb friction surfaces with varyingcoefficients of friction. The region above each of these curves is the stable region. The‘Zero Friction’ limit curve is a vertical line for a zero-friction surface. At the otherextreme, an peg in a hole would create a horizontal line for an infinite friction surface.The intermediate surfaces represent smooth and rough surfaces such as ice on ice andrubber on asphalt.low resistance to movement since the bearings are designed to roll with little friction.Though the bearing forces are complex, we will assume that increasing normal forceon the skateboard adds to the rolling resistance. For forces along the short axis ofthe skateboard, the limit curve along that axis is determined by the coefficient offriction between the urethane wheels and the concrete surface. This gives a limitsurface that is not rotationally symmetric about the normal force axis. The naturalgecko adhesive, due to its structure, also does not exhibit a surface that is rotationallysymmetric.2.2.2 Embedded Cone ModelTo include the effects of adhesion, an old and simple model known as the embeddedcone model captures much of the behavior. This model simply subtracts an offset
CHAPTER 2. BACKGROUND 11stableunstableFigure 2.6: Embedded cone limit curve. The gray area indicates pairs of normal andshear forces at the adhesive interface that remain attached. Pairs of forces below thered limit curve will result in the breaking of the adhesive interface. The α indicatesthe maximum tensile normal force that the interface can withstand. Note that incontrast with the coulomb surface, that there are areas within the stable area thatcan withstand normal tensile forces.from the coulomb friction limit surface [4, 5].F N = 1 µ |F S|− αThe limit surface now includes the origin and regions with negative values of F N .As we did with the ice and asphalt, we can conduct a thought experiment toenvision limit curves including adhesion. Consider for example a frictionless refrigeratormagnet. Any amount of shear force will result in interface failure and relativemovement. The limit curve is then only a line along the normal force axis that extendsfrom infinite compression to the strength of the magnet in tension. As we addfriction to the interface, the slopes will reduce in magnitude as we saw for the ice andasphalt examples. If we place this magnet on the end of the dowel from our previous
CHAPTER 2. BACKGROUND 12Zero FrictionLow FrictionHigh FrictionInfinite FrictionFigure 2.7: These four limit curves depict embedded cone surfaces with varyingamounts of shear friction but equal amounts of maximum normal capacity. Thezero friction limit curve is a fictional, frictionless magnet that withstands no shearforce but some tensile normal force. Low and high friction curves correspond to amagnet with either low or high friction. The infinite friction curve could be the resultof a peg in a hole attached by adhesive at the bottom.examples, we will have a limit surface that is a line parallel with the shear force axis.2.2.3 Savkoor Briggs ModelThe adhesive behavior exhibited by pressure sensitive adhesives is also observed inthe contact of hemispherical surfaces. Savkoor and Briggs introduced a model forhemispherical contacts that accounts for the shear and normal forces and their interaction. The Savkoor-Briggs theory is an extension to earlier theories on theinteractions between hemispherical surfaces [7, 8]. The Hertz theory  treated thedeformation of hemispherical surfaces in the presence of compressive forces but in theabsence of attractive surface forces. The JKR theory  extended the Hertz theory toinclude attractive surface forces. The JKR theory predicts a finite adhesion force fora hemisphere in contact with a plane dictated by the surface energy of the material
CHAPTER 2. BACKGROUND 13(γ) and the radius (R) of the hemispherical surface.F N = − 3 πγR (2.2)2This JKR prediction for the force at detachment of a fibril is widely used but doesnot account for shear stress. The Savkoor-Briggs theory extends the JKR theory byaccounting for the presence of shear stress at the adhesive interface. In this analysis,the shear force causes a reduction of the radius of contact predicted by JKR theoryand thus a reduction in the normal direction adhesive force.plotted as a limit surface to reveal, instead of a cone, a parabolic surface.Their model can beThe Savkoor-Briggs model provides an expression for F N as a function of F S . Itis a parabolic function with a y-intercept of − 3 γπR, the JKR pulloff force for zero2shear:F N =Kλ32γπR F 2 S − 3 2 γπRWhere Kλ forms a dimensionless factor that takes into account the shear modulusand bulk modulus of the material and ends up being a function of the Poisson’s ratioof the material. For a polymer ν = 0.5, Kλ = 8 and the normal force at failure isgiven byF N = 14γπR F 2 S − 3 2 γπRWe see that like the embedded cone model, the maximum normal adhesive forceoccurs when the shear force (F S ) is zero.2.2.4 Frictional Adhesion Limit SurfaceThe limit surface displayed by the gecko (Figure 2.8) is unlike the embedded coneor Savkoor-Briggs limit surfaces that describe pressure-sensitive adhesives. It insteadfollows a model termed frictional adhesion . The first clear difference is that thefrictional adhesion surface exhibited by the gecko is not symmetric about the origin.Another important difference is that the frictional adhesion limit surface crosses
CHAPTER 2. BACKGROUND 14through the origin. Since the limit surface crosses the origin, that means that forcesof relatively low magnitude can release the adhesive depending on the direction ofthe force. The asymmetric limit surface reflects the fact that the gecko’s adhesivestructure is also asymmetric. This anisotropic or directional behavior is one of theproperties we want to replicate in our fibrillar adhesives. Were we to add a dimensionin our force space for forces in the transverse direction, we would have axes for F N ,the normal force, F S , the shear force, and F T , the transverse force, and we would seethat the gecko surface is symmetric about the F N − F S plane. We could equivalentlysay that the limit surface is an even function of the transverse force. The asymmetrymeans that in one direction the gecko adhesive behaves like a coulomb-friction surfacewhile in the other direction the adhesive behaves in a very novel way. As Figure 2.8shows, as the amount of shear stress at the interface increases, the amount of normalstress that the interface can withstand is increased. This is an advantageous propertyfor an animal that climbs vertical surfaces. The natural application of shear stressdue to the weight of the animal will result in the ability to withstand moments thatarise because the animal’s center of gravity is away from the wall. This stress willincrease while the animal is in motion and the stability of the interface will increase. This frictional adhesive property is very advantageous for climbing and was aproperty we wanted to achieve in our fibrillar adhesive.2.3 Previous LiteratureThere have been many attempts in the literature to make adhesives inspired by thegecko adhesive. The work described here is distinguished by our objective of creatingan adhesive that will be well suited for climbing. This means that the gecko propertiesof anisotropy and frictional adhesion are important while other properties of the geckoadhesive such as multilevel hierarchy and nanometer terminal feature dimension maynot be necessary. A brief summary of the gecko-inspired adhesives relevant to thiswork follow.There have been many demonstrations of fibrillar adhesives made from materialsthat do not fulfill the Dahlquist criterion [11, 12, 13, 14, 15]. Commonly used materials
CHAPTER 2. BACKGROUND 15stableunstableFigure 2.8: Frictional adhesion limit surface showing increased normal adhesive stabilitywith increased shear stress. The grey area shows regions of stable attachmentwhile the white areas below the curve are unstable areas where the adhesive will detach.The arrow on the force space graph shows the projections of the gravity force onthe shear force and normal force axes. The positive F N direction denotes compressivenormal stress at the interface.
CHAPTER 2. BACKGROUND 16in the literature are elastomeric polymers [16, 12], carbon nanotubes [13, 17, 18], andthermoplastics . The initial gecko-inspired adhesives exploited the principle ofcontact splitting  to create fibrillar adhesives that demonstrated adhesion in thenormal direction. This contact splitting principle states that increasing the numberof terminal features leads to improvement in adhesion.These first fibrillar structures were simple pillars,  fabricated from polymethylmethacrylate(PMMA). These pillars were approximately 200 nm in diameter and2 µm tall. The contact splitting principle has been taken to an extreme by researchersusing carbon nanotubes [13, 17, 18]. The size and density of carbon nanotube arraysexplain why they often report adhesion in excess of the gecko.Going beyond contact splitting, researchers investigated the role of tip shape,adding structures to the top of the pillars to enhance adhesion [16, 12, 21]. The firstof these tip structures often had cylindrical symmetry and formed a flat termination atthe top of the pillar. These tips generally enhanced adhesion in the normal directionbut were not usually tested for shear force generation or anisotropy. Gorb et al. found that these tips often led to poor shear force performance. This was due to thefact that when the pillar bent under shear load, the surface area available for contactwas reduced.Inspired by the slanted hair architecture in many of the animals that use fibrillaradhesives, researchers began fabricating structures that were angled with respect tothe backing layer [22, 23]. These structures began to show interesting interactionsbetween the levels of shear and normal adhesion. Researchers using very slenderfibrils (100 nm scale), often found that after repeated use or intentional training, thefibrils would take on a predominant orientation, affording the adhesive anisotropicqualities [17, 19].The work presented here was motivated by the desire to create an adhesive thatpossessed the gecko-like behavior necessary for climbing. This included the frictionaladhesion property and the anisotropic adhesion. The fabricated structures in thiswork are inspired by previous work on gecko synthetic adhesives  as well as workon slanted micro-structures using SU-8.In this work we also designed a structure that was asymmetric. A key distinction
CHAPTER 2. BACKGROUND 17in this work is that we envisioned an adhesive structure that would change shapebased on the amount of loading and that this change in shape would affect the adhesiveproperties. This asymmetrical structure has a sharp angled tip that allows theadhesive to present a variable surface area based on the amount of loading.
Chapter 3Fabrication3.1 Design PrinciplesThis fabrication process drew inspiration from the adhesive structure of the tokaygecko [25, 26] and previous work [27, 28, 29, 30] on making angled microstructuresusing SU-8, a photosensitive epoxy. We envisioned a structure that would deformunder compression to increase the surface area and achieve the frictional adhesionobserved in the gecko.The SU-8 material had been used successfully to fabricate high-aspect ratio structuresso it was our choice for the photosensitive polymer mold material. Issues ofease of use and material compatibility led us to the choice of silicone rubber as thematerial we would cast and create the pillars with. Urethanes were also consideredbut because of material incompatibility, they would not cure while in contact withthe SU-8 material.3.2 OverviewThis adhesive was created using a molding process. The reusable mold was createdusing SU-8 on a quartz wafer with a unique lithography process. The mold has anarray of wedge-shaped pits. A two-part exposure process was used. The first exposurewill create the vertical wall of the mold and the second will create the slanted wall.18
CHAPTER 3. FABRICATION 19We then vacuum cast and cure polydimethylsiloxane rubber (PDMS) in the mold andpeel out to release. This process flow is depicted in Figure 184.108.40.206 Mold3.3.1 Metal DepositionTo create the mold, we deposited and patterned a thin layer of aluminum on a doublepolished quartz wafer to create a hardmask. The mold is fabricated using a doublepolishedtransparent 100 mm quartz wafer. The wafer was cleaned using the RCAclean with a sulfuric acid and hydrogen peroxide bath to remove organic materialfollowed by a hydrogen peroxide and hydrochloric acid bath to getter metal ions.We then sputter deposited a 100 nm film of aluminum onto the wafer. Then weperformed a standard SNF photolithography process, using 1.0 µm of Shipley 3612photoresist. This layer of photo resist was exposed with 19.5 mW/cm 2 of ultravioletlight on a contact aligner to create the pattern. The photoresist was developed andthe aluminum was etched in a wet bath of phosphoric acid, acetic acid, and nitricacid. The photoresist was removed using a bath of PRX-127 at 40 ◦ C for 20 minutes.This aluminum layer served as a mask for the SU-8 layer in a later processing step.3.3.2 SU-8 DepositionWe then spin coat and bake a layer of SU-8 on the side of the wafer that has thealuminum surface. First, the wafer was cleaned with isopropyl alcohol and then singedat 110 ◦ C for 5 minutes to drive off moisture. Approximately 5 mL of SU-8 2035 wasdrawn into a syringe from the bottle. The wafer is placed on a vacuum chuck spinnerand the SU-8 was dispensed on the wafer center. During the dispensing stage, carewas taken to avoid creating bubbles trapped in the viscous SU-8. The wafer was thenspun at ∼1000 RPM for 30 seconds to planarize the SU-8 at a target thickness of80µm. The wafer was then baked to drive excess solvent from the SU-8 film. Care wastaken to ensure even heating of the SU-8 to achieve a uniform thickness film. We useda plate of aluminum with a machined flat surface to make good thermal contact with
CHAPTER 3. FABRICATION 2012367458QuartzAluminumPDMSUnexposed SU8Exposed SU8Figure 3.1: Fabrication Sequence 1) Deposit aluminum on quartz wafer 2) Patternaluminum to create self-aligned mask 3) Deposit SU-8 on top of aluminum 4) Angledself-aligned UV exposure from backside 5) Align mask to topside and UV expose6) Develop 7) Cast and spin PDMS 8) Peel out cast MicroWedges and backing layer
CHAPTER 3. FABRICATION 21the hot plate. This provided better contact than the aluminum foil usually placedover the hotplate. We cleaned this plate to remove SU-8 transferred from earlierprocesses. The wafer was baked on this aluminum plate, starting at 65 ◦ C with a slow(5 minute) ramp to 95 ◦ C. The wafer was then held at 95 ◦ C for 13 minutes.Special care was exercised during this part of the process. It is during this stepthat problems in the planarity of the SU-8 would arise. Generally, depressions, wouldform in the SU-8 often with a small bubble visible at the bottom of the depression.These depressions negatively influenced the yield of the adhesive.3.3.3 First SU-8 ExposureWe first performed a planar exposure using a contact aligner. The quartz maskwas aligned with the hardmask layer to provide registration between the verticaland slanted features. After alignment, the SU-8 was exposed to 200 mW/cm 2 ofUV energy. On the Karl Suss contact aligner in the SNF facility, this exposure wasperformed in 2 equally timed steps (6.9 sec) separated by 10 sec. This exposurewas performed with a long-pass filter (PL 360-LP Omega Optical) to block radiationshorter than 350 nm.3.3.4 Second SU-8 ExposureAfter the first exposure, the wafer was placed on a tilted exposure stage. We adjustedthe stage, correcting for the index of refraction of the SU-8, to achieve the desiredangle for the slanted surfaces of the mold. In this work we chose the pillar faceangle to be 14.8 ◦ giving the wedges a 4:1 aspect ratio. We then exposed the waferto ultraviolet light from the underside. The dosage used was 184 mW/cm 2 of UVenergy in two equal doses (4.0 seconds) separated by 10 seconds. This exposure wasperformed under a collimated UV illumination system, taking advantage of the nowself-aligned hardmask layer of aluminum.
CHAPTER 3. FABRICATION 223.3.5 SU-8 Cure and DevelopThe SU-8 was then baked and developed using standard processes found in the SU-8application notes. We baked the SU-8 on a hotplate for the chemical amplificationof the photoresist. The bake started at 65 ◦ C and was ramped to 95 ◦ C and then heldat 95 ◦ C for 7 minutes. The wafer was allowed to cool and then placed in a beaker ofdeveloping solution for approximately 9 minutes. We agitated the wafer occasionallyand inspected for complete development of the SU-8 film. The wafer was then given a100 ◦ C postbake for 5 minutes to harden the resist and prepare it for the temperaturesit would experience during the molding process. At this point the mold was completeand ready for use in casting. Figure 3.2 shows a photograph of the transparent moldin a wafer container.3.4 Casting ProcessWith the mold complete, we used it to cast a PDMS sample. The PDMS (DowCorning Sylgard 170) is a two part mixture. Equal mass portions were combined andmixed thoroughly. The mixed and uncured PDMS was placed in a vacuum chamberwith the SU-8 mold wafer. The chamber was evacuated and air trapped in the PDMSwas liberated. Still under vacuum, the PDMS was poured on the wafer. Air trappedin the mold bubbled through the PDMS and was removed to prevent voids. We thenremoved the mold from vacuum and spun it to planarize the PDMS backing to thedesired thickness. Our backings were in the range of 300 µm to 1200 µm. The PDMSwas cured in an oven at 85 ◦ C for 15 minutes. The adhesive pillar arrays were releasedby gently peeling the backing layer from the mold. Figure 3.3 shows the PDMS layerafter release from a mold. From these layers of PDMS, we cut samples and mountedthem on glass slides for measurements. Figures 3.4 and 3.5 show SEM images of theresulting adhesive pillars.
CHAPTER 3. FABRICATION 23Figure 3.2: Photograph of complete SU-8 on quartz wafer mold.indicate arrays of different sized structures on the wafer.Different colors
CHAPTER 3. FABRICATION 24Figure 3.3: Photograph of adhesive pillar array as released from mold. PDMS is castinto the mold and cured and then peeled from the mold.
CHAPTER 3. FABRICATION 25Figure 3.4: SEM image of adhesive pillar arrays. The left edge of the three foregroundpillars is vertical and the right edge of these pillars is slanted at approximately 14 ◦ .
CHAPTER 3. FABRICATION 26Figure 3.5: SEM profile view of adhesive pillar arrays. The vertical and slanted facescan be seen, as well as the tip of the structure. The thickness of the backing layer isalso clearly visible and is equal to the height of the stalks.
CHAPTER 3. FABRICATION 273.5 Process IssuesTo characterize this process as high-yield would be misleading. Though we couldoften create large areas of well defined pillars (at least 1 cm 2 with no obvious defects)often molds were unsuccessful.This section will cover the process problems that we encountered.3.5.1 SkinningOne especially vexing problem was that during the develop process, a film would formover the top of the mold. The reason for this layer was not determined. This causedtwo problems. The first problem is reduced yield due to having a reentrant aperture.Figure 3.6 shows a SEM image of this thin layer and adhesive pillars that did notcompletely release as a result. The second problem is that this leads to an overhangthat causes the pillar to sit atop a narrower pedestal. Figure 3.7 shows a SEM imageat the base of the pillar showing this narrowing. This introduces an extra complianceat the base of the pillar that affects the mechanics of the pillar. This compliance atthe base will result in less bending across the beam, affecting the adhesive behavior.3.5.2 ScallopingAnother area where the incomplete development of the mold caused noticeable variabilityin the structures was at the tip of the mold. In a feature reminiscent of ”grass”in deep reactive ion etching processes, thin membranes of SU-8 remain in the bottomof the mold where the adhesive tip is formed. Figure 3.8 shows these high-aspect-ratiostructures at the bottom of the mold. Figure 3.9 shows the resulting tip.3.5.3 Alignment IssuesThe process to create a slanted face and a vertical face involves an alignment through a60-100 µm layer of SU-8. This distance is well beyond the depth of field in the opticalsystem of our mask aligners at the fabrication facility. This necessitates the use ofdigital image capture alignment techniques and creates difficulty and uncertainty in
CHAPTER 3. FABRICATION 28Figure 3.6: SEM image of overhanging film closing off the mold. This mold hashad PDMS cast and partially released from the mold. Pillars are visible that havepartially released before tearing as well as pillars that remain completely in the mold.
CHAPTER 3. FABRICATION 29Figure 3.7: SEM detail image of the base of an adhesive pillar showing the undercutdue to the overhanging film shown in Figure 3.6. This undercut affects the bendingcompliance of the pillar.
CHAPTER 3. FABRICATION 30Figure 3.8: SEM image of incomplete development in the bottom of a mold cavity.Image shows sheet like structures at the tip of the mold cavity that lead to a roughenedtip.
CHAPTER 3. FABRICATION 31Figure 3.9: SEM image of roughened tip due to incomplete mold development.
CHAPTER 3. FABRICATION 32the alignment process. The critical dimension of alignment is in the direction from thefront slanted face to the back vertical face. This direction is from crown to flat on thewafer. If there is misalignment in the direction of the crown, the opening may reachthe bottom of the SU-8, resulting in a truncated tip. If instead the misalignmentis in the direction of the wafer flat, the mold feature will be more shallow. If themisalignment is great enough, an undeveloped region of SU-8 can be exposed at thesurface. Figures 3.10 and 3.11 show what appears to be undeveloped SU-8 escapingto the surface after a misalignment. These figures also show that the feature is notas deep as expected, which is a consequence of misalignment.3.5.4 Going ForwardThis SU-8 process has provided a valuable prototyping platform for these asymmetricadhesives. It is not a robust process and the mold does not have a long lifetime sincethe SU-8 layer is prone to delamination and cracking. Efforts to create a mold froma more robust material would be worthwhile. There are efforts underway to exploremicro-indentation as a tool. Adhesives have been attempted using micro-indentation but did not yield high-aspect-ratio structures. If a robust mold could be madeusing this method, it would be a large benefit to the yield and reusability of thematerial.
CHAPTER 3. FABRICATION 33Figure 3.10: SEM image of misalignment allowing the escape of undeveloped SU-8during the development process. Under the spherical bubbles there is a seam visiblethat exposes a volume of unexposed SU-8.
CHAPTER 3. FABRICATION 34Figure 3.11: SEM image detail of undeveloped SU-8 escaping to the surface of themold.
Chapter 4Pillar Array TestingThe principal objective in the force testing of these adhesive arrays is to determinehow the array behaves when subjected to combinations of shear and normal force. Ofparticular interest is the combination of shear and normal load that leads to failureof the interface. By mapping out the combinations of forces that cause failure, wecan construct a region that the stresses must stay within to ensure stable attachment.Pressure-sensitive adhesives are generally applied with a compressive normal load beforetensile stress is applied to the interface. We attach these fibrillar adhesives in asimilar manner. This is achieved by bringing the adhesive and a surface for attachmentinto compressive contact to initiate the adhesive bond and then withdrawingthe surface in a range of directions to create tensile stresses with varying componentsin the normal and shear directions. By using a force sensor that can simultaneouslymeasure the shear and normal forces at the interface, we can determine these forcepairs that bound the stable and unstable regions. These forces are plotted in a limitsurface to visualize the pairs of forces for which stable attachment is possible.4.1 Test PlatformWe tested the adhesive arrays on a custom built force testing apparatus  with athree-axis motor stage to control friction and loading at arbitrary angles. A photo ofthe test apparatus can be seen in Figure 4.2 and a block diagram in Figure 4.3. The35
CHAPTER 4. PILLAR ARRAY TESTING 3690°45°substrate0°force plateFigure 4.1: Limit surface test diagram showing the conventions for force and directionin our force testing setup. The arrows indicate the direction of positive force appliedto the force plate. The unlabeled allow is meant to illustrate the direction of thesubstrate during the compressive phase of the trajectory. The arrows at 90 ◦ 45 ◦ and0 ◦ are the different retraction angles for the tensile phase of the trajectory. The 90 ◦retraction will cause mostly normal stress while the 0 ◦ will create mostly shear shearstress. These different angle and the resulting mix of normal and shear stress allowus to plot the limit curve.
CHAPTER 4. PILLAR ARRAY TESTING 37setup is capable of moving a flat glass substrate and sample into and out of contactalong trajectories in both the normal and tangential directions simultaneously. Theapparatus consists of a 3-axis linear stage, force transducer, and 2-axis manual tiltstage. The motion stage (Velmex, MAXY4009W2-S4 and MA2506B-S2.5) has a 10µm positioning resolution in the tangential direction and a 1 µm positioning resolutionin the normal direction. A flat glass substrate was attached to the motion stage andthe sample is placed upon a 6-axis force/torque sensor (ATI Industrial Automation,Gamma Transducer SI-32-2.5) with an accuracy of approximately ± 25 mN. Theforce transducer was mounted onto a manual 2-axis tilt stage (Newport, 30 Series TiltPlatform) which was used for manual alignment of the sample relative to the substrate.This alignment is somewhat unique since many researchers use hemispherical lensesto avoid alignment issues. Despite the difficulties that accompany alignment, wedecided to use a flat surface since it best simulates the intended application of theadhesive (a climbing robot on vertical smooth surfaces). The stage was controlledby a custom microcontroller. Displacement instructions were sent from a Labviewapplication running on a Windows XP system to the microcontroller over a serialconnection. The microcontroller updated the stepper motors at a rate of 1 kHz.Force and position data were collected at a frequency of 1 kHz. Force data fromthe force sensor and displacement information from the stages were sent back to theLabview application and written to text files for later analysis. Data were analyzedusing Matlab (The Mathworks, Inc.).4.2 Testing ProcedureAn array of adhesive of dimension ∼1 cm 2 was mounted on a glass slide. Since thebacking of the adhesive was smooth, the backing will adhere to the glass slide. Thisglass slide was fixed to the load cell using a conventional tape adhesive. A camerawas used to observe that the sample was coplanar with the flat glass substrate. If thesample and glass substrate are misaligned, it will be possible to have some pillars insevere compression, while not contacting other pillars. This coplanarity was difficultto achieve since the sample has non-uniform backing thickness and pillar height.
CHAPTER 4. PILLAR ARRAY TESTING 38Figure 4.2: Limit surface testing apparatus. The camera objective used for alignmentis visible at the top of the photo. Below the camera objective is the arm and glassplate. This glass plate makes contact with the adhesive affixed to the aluminumpedestal below the plate. Underneath the large grey plate is the load cell with thesignal cable in front. The goniometers can be seen beneath the load cell atop the verticalpedestal. The arm and pedestal, while not ideal, are necessary to accommodatethe large stages used for motion control.
CHAPTER 4. PILLAR ARRAY TESTING 39Substrate3-Axis StageForceSensorMicroprocessorBoardAlignmentControlComputerFigure 4.3: Force measurement apparatus block diagram depicting the signal flow inour system. The alignment control is manual and has no link to the computer. Thecomputer sends locations and velocities to the custom microprocessor board whichthen drives the 3-axis stage. Stage encoder data for position feedback is returned tothe computer through the microprocessor board. The force sensor data is fed directlyto the computer. The computer runs a LabView application which coordinates thedata.
CHAPTER 4. PILLAR ARRAY TESTING 40Our approach was to use a camera to view the sample as it comes into contactwith the glass substrate. When the wedges made contact with the glass surfacethe reflectivity of the bottom glass surface was enhanced and the areas of contactappear bright. The sample is brought slowly in and out of contact and when thiscolor change occurs evenly across the sample we consider the sample aligned. Wealso took care to manually position the sample so that the rows of adhesive pillarswere parallel to the direction of stage travel. This also was verified through theoverhead camera. To specify the trajectory of compression and tension in the tests, wespecified the distances and speeds at which the stage would move in software. Theseinstructions were stored in the LabView application to be sent to the microcontrollerat run time. With the sample fixed and aligned and the trajectories specified, thetest apparatus runs and collects data. Figure 4.1 shows the angles and axes of theforces measured relative to the adhesive and the force transducer. These tests weredisplacement controlled. The amount of compression was specified by the distancethat the stage travels in the normal direction after the initial contact. This initialcontact position was defined as the point at which normal force due to compressionis recorded. Generally the maximum compression distance was on the order of halfof the pillar height, in this case approximately 40 microns. Once compression wasfinished, the glass surface was withdrawn at a velocity of 1000 µm/sec.4.2.1 Data AnalysisData was compiled, scaled, and then plotted. A plot of the data as collected lookslike Figure 4.4. Failure points were identified using the max-power method . Themax power method defines the point during tensile loading where the dot productbetween the interface force and the velocity of the glass stage is a minimum. That is,t f , the time of the failure is defined to beF (t f ) · v(t f ) ≤ F (t) · v(t), ∀t. (4.1)The shear and normal forces at the identified failure point were recorded for eachof the trajectories. When we look at the data we see that failure is usually indicated
CHAPTER 4. PILLAR ARRAY TESTING 41by changes in the slope of the force vs. time curves during the tensile phase of thetrajectory. These changes in the force indicate transitions from static to kinetic ordynamic friction and release events. Figure 4.4 shows a failure when the substratewas withdrawn at an angle parallel to the interface (0 ◦ according to Figure 4.1). Theblack x marks depict the failure point predicted by the max power criterion. Thereare slope changes before the failure point shown but these slope changes were duringthe compressive phase and do not represent relative movement. The force trace plot(Figure 4.4) allows us to see the forces exerted by the adhesive as a function of time.The plot shows that dynamic sliding adhesion is obtained where despite slipping,both shear and normal adhesion forces are exerted. In this test, the adhesive wasable to simultaneously maintain 2 kPa of adhesion and 8 kPa of shear. This impliesthat individual hairs that have detached are able to reattach and exert adhesiveforce. This property allows the adhesive a graceful failure mode desirable for roboticsor locomotion applications. Other GSAs have demonstrated similar results using aspherical surface with a radius of ∼5 mm . These tests using spherical glasssurfaces don’t necessarily demonstrate the reattachment of fibrils since only a portionof the sample’s fibers are in contact. This is in contrast with the testing describedhere, where the glass surface has a larger area than the adhesive sample and all theadhesive fibers are available for adhesive contact.Figure 4.5 shows the force trace when the substrate is drawn vertically away fromthe microwedge adhesive (90 ◦ according to Figure 4.1). In this case the failure pointpredicted is not at the precise moment of the failure, but the forces reported areessentially the same. This is a minor shortcoming of the max power method. Weinspected the data to be sure that each of the failure points reported appear to becorrect. To construct the limit curve, the adhesive is tested at multiple compressiondepths and angles of withdrawal. Three tests are conducted at each compressiondepth and angle. The failure points are computed in each of these tests and compiledto construct a limit curve.
CHAPTER 4. PILLAR ARRAY TESTING 42Figure 4.4: Adhesive array force trace with parallel (0 ◦ ) retraction. The normaltrace shows the initial compression phase followed by a region of adhesion during theparallel drag. In the shear trace, we see that there is a shear force created by theadhesive at the same time as the normal adhesion force. The failure point occurs atthe black x mark. At the time of failure, the shear (lateral) and normal forces arerecorded and plotted as a pair in the limit curve.4.3 ResultsFigure 4.6 shows the resulting limit surface from a fibrillar adhesive sample. Thelimit surface in Figure 4.6, obtained through many trials over a range of preloadangles, preload depths, and exit angles, is a map of the release points for differentshear to adhesion ratios. We notice that the surface crosses the origin and has anegative slope as it leaves the origin. As discussed in Section 2.2.4, this negativeslope indicates that the normal stress capacity of the adhesive is increased by theapplication of shear stress at the interface. The limit surface also shows that force
CHAPTER 4. PILLAR ARRAY TESTING 43Figure 4.5: Adhesive array force trace with vertical retraction. The compressionphase can be seen in the normal trace beginning near 120 msec and ending near 150msec. During the tensile phase, this force is reduced and falls to zero. We see that thestresses during the retraction or tensile phase in this case are primarily in the normaldirection. It is also clear that at the time of failure there is little or no adhesive force(negative normal interface stress).pairs very close to the origin can result in detachment. This means that when theshear stress is removed from the interface, the adhesive can be removed with verylittle force. The increase of normal force with the application of shear force saturatesat a shear force corresponding to ∼13 kPa of shear stress. Above this level, the normalholding power is reduced and at ∼18 kPa of shear stress, the interface can only bemaintained if there is compressive normal force at the interface. A more detaileddiscussion of these array results can be found in  and .As a control, we tested a flat thin sample of PDMS rubber to determine its limitsurface. The limit surface of the flat control in Figure 4.7, shows behavior similar
CHAPTER 4. PILLAR ARRAY TESTING 4410Normal Stress (kPa)50−5−100 5 10 15 20 25 30Shear Stress (kPa)Figure 4.6: Limit curve for adhesive pillar array. Each plot point represents anadhesive failure. The points in force space above the line described by the pairs arestable while points below the curve will detach. We see that the adhesion is increased08 Jul 2010 - 18:15as the shear/Users/dsoto/current/cabroncito/20sBL1_1/code/plotLimitSurface.pyincreases. Also, if the shear is decreased to zero, the adhesion is reducedand the adhesive can be removed with limitSurface.pdf very little force.to the embedded cone model (discussed in section 2.2.2) where increasing shear decreasesthe available normal force. Also, the limit surface of the flat control does notpass through the origin. This implies that there must be a normal force exerted atdetachment when there is no shear and that there is no detachment possible withoutthe application of tensile stress to the interface. It should be noted that the maximumnormal stress achieved is 2 times greater for the flat control sample. This reminds usthat our choice of adhesive depends on the specific behavior we desire.
CHAPTER 4. PILLAR ARRAY TESTING 453020Adhesion (kPa)100−10−20−40 −20 0 20 40 60Shear (kPa)Figure 4.7: Limit curve for PDMS flat control sample. We tested the material used forthe adhesive pillars by creating a flat sample and testing. Each plot point representsan adhesive failure. This curve has a different character than Figure 4.6. This limitcurve does not intersect the origin and increasing shear leads to diminished adhesivecapability.
Chapter 5Single Pillar TestingThis chapter describes the testing performed on single isolated pillars from the adhesivearrays. In Chapter 4 the adhesive properties of arrays of tapered adhesive pillarsare discussed. Having accumulated this body of data on the behavior of these pillarsin arrays, we became interested in the behavior of single elements. We set out todetermine what aspects of the adhesive behavior are intrinsic to the wedge structuresand what aspects are emergent in these large arrays. To measure the behavior ofsingle isolated pillars, we use a system with similar capabilities to the array testingsystem, but with µN force resolution. This system allows us to observe behaviorthat is not evident in arrays of thousands of pillars. We also performed testing ofnontapered pillars to understand the role that the pillar shape plays in the adhesiveproperties.5.1 Force Measurement System Description5.1.1 Dual Axis CantileverThe central part of this force measurement system is a force transducer capable of µNresolution force measurement. In the array testing apparatus we used a commerciallyavailable force sensor with mN resolution. In this case, the force sensor is a dual-axismicromachined force sensor as described in [35, 36]. This flat-tipped piezoresistive46
CHAPTER 5. SINGLE PILLAR TESTING 47Figure 5.1: SEM image of dual-axis cantilever. Normal force is in the out of planedirection. The normal force piezoresistors are located in the two short members atthe base of the triangular tip. The shear force is in the horizontal direction. Thefour slender structures deflect together. The shear force piezoresistors are locatedat the base of the inner two structures. The thickness is reduced in those areas toconcentrate the stress.cantilever is capable of simultaneously measuring forces along two orthogonal axesto measure the forces at the adhesive interface. An electron microscope image ofa representative cantilever is shown in Figure 5.1. This sensor is a microfabricatedsilicon cantilever with implanted piezoresistive regions that form strain sensors thatchange resistance when the cantilever is deflected. These piezoresistive regions aredepicted in a rendered illustration of the cantilever in Figure 5.2. It is similar to anatomic force microscope (AFM) cantilever but instead of a sharp tip, this sensor has a20 µm by 40 µm platform for the pillar to adhere to and its unique geometry enablessimultaneous detection of normal and shear forces applied at the tip.The change in resistance is sensed by a Wheatstone-bridge signal-conditioningcircuit and converted to a voltage. The structure is designed so that the members
CHAPTER 5. SINGLE PILLAR TESTING 48lateralsensorsnormalsensorsPiezoresistorsFigure 5.2: Rendered illustration of the dual-axis cantilever. The locations of thenormal and lateral force piezoresistive sensors are indicated on the illustration.used to sense normal forces are stiff in the shear direction and vice versa to minimizecrosstalk between the two axes. To calibrate the sensor, we measure the displacementsensitivity of the cantilever and signal-conditioning circuit directly, and then estimatethe cantilever’s stiffness using a combination of resonant frequency measurement,finite-element modeling, and interaction measurements with a reference cantilever. The spring constants of the cantilevers vary from 0.3–0.6 N/m in the normaldirection and 0.3–3.0 N/m in the lateral direction. The values of these stiffnessesof the two cantilevers most often used for this testing are shown in Table 5.1. Itis important to note that these stiffnesses are within an order of magnitude of thecorresponding stiffnesses of the pillar structures. This is in contrast with the arraytesting setup where the difference between the normal stiffness of the array and theforce plate is about a factor of 200. When the data is interpreted, special attentionmust be paid to account for the deflection of the dual-axis cantilever during testingsince the compliances are similar.
CHAPTER 5. SINGLE PILLAR TESTING 49Cantilever k N (N/m) k S (N/m) s N (V/µm) s S (V/µm)529b02 0.659 3.898 0.224 1.148629a03 0.313 0.307 0.148 0.473Table 5.1: This table shows the stiffnesses and displacement sensitivities for thecantilevers used in these measurements. k n is the normal spring constant of thecantilever and k l is the lateral or shear spring constant. s N is the normal sensitivityof the cantilever circuit at the nominal gain and s S is the shear sensitivity.5.1.2 Force Measurement SystemThe measurement is performed in a method very similar to the array measurement.We have tilt stages for alignment, an actuated stage for positioning, and a forcetransduction element. To characterize the adhesive properties, we determine the setof shear and normal force pairs for which stable attachment is possible. A photographof the system is provided in Figure 5.3.The stage that provides motion is a piezoelectric actuator (P-731.20, Physik Instrumente).Typical load drag pull trajectories are executed and the resultant forcesare stored on a computer for analysis. These plots show the normal and lateral forceson the dual-axis cantilever during contact with the adhesive pillar.The adhesive pillar and cantilever are placed in a custom system that allows foralignment of the pillar and cantilever, motion control, and force data collection. Thedual-axis cantilever is mounted to a piezoelectric stage (P-731.20, Physik Instrumente)with capacitive position sensors (E-509.C2, Physik Instrumente) to providemicron-scale positioning of the cantilever relative to the fibril under test. The cantileveris mounted and wirebonded to a surface-mount breakout board and a cablewas attached. These leads are sent to a signal-conditioning circuit based on a Wheatstonebridge to monitor the resistance change in the piezoresistive strain sensors.A data-acquisition board (PCI-6052E, National Instruments) is used to output theanalog signal to the piezoelectric stage and to acquire the analog signals from thecapacitive position feedback and the Wheatstone bridge. These signals are controlledand tabulated by a software application (Labview, National Instruments) running ona desktop computer running Microsoft Windows XP. Figure 5.4 provides a schematic
CHAPTER 5. SINGLE PILLAR TESTING 50Figure 5.3: The force measurement apparatus for single adhesive pillar measurements.The microscope objective for viewing is at the top of the photo. The black box onthe right is the piezoelectric stage. The aluminum arm and block holds the cantileverand circuit board at the center of the photo. The black wire runs the signal backto the signal-conditioning circuit. On the left are the positioning stages to allow forsix-axis positioning relative to the cantilever surface.
CHAPTER 5. SINGLE PILLAR TESTING 51AlignmentControlMounting PinComputerCantileverAmplifierPiezoAmplifierCantileverPiezoelectricStageFigure 5.4: Single adhesive pillar apparatus block diagram.representation of these connections.The adhesive is mounted at the end of a steel pin. The pin holder has five degrees offreedom to provide alignment and adjustment relative to the plane of the cantilevertip. Any adjustments needed in the sixth degree of freedom are made by gentlybending the mounting pin.5.1.3 Sample PreparationIsolated stalks were mounted using two different sources. The first sources were moldsthat, owing to clogging and other degradation, had sparse coverage of stalks whencast. We later fabricated molds that had custom fabricated stalks with sufficientspacing to make manual isolation simpler.Using either of these types of molds, isolated hairs are identified and then cutfrom the backing using steel razor blades that are cut and ground to allow for better
CHAPTER 5. SINGLE PILLAR TESTING 52viewing under the dissection stereomicroscope. Sample sizes are on the order of 200µm by 200 µm. For mounting, a steel pin was prepared by tapering the flat side ofthe pin until the tip diameter was on the order of the sample size. Cyanoacrylateadhesive was used to fix the pin to the sample. Samples were allowed to cure forat least an hour before testing. A mounted sample and the dual-axis cantilever areshown in Figure 220.127.116.11.4 Limit Curve TestA single pillar limit curve was plotted by performing multiple trajectories on a singlewedge that simulate loading of the adhesive under use. By withdrawing the cantileverat different angles, we can achieve varying ratios of normal to shear adhesive forceand can map out a limit curve.Figure 5.6 shows the relative orientations of the cantilever and pillar, the conventionfor forces on the cantilever, and the directions of pillar motion during the test.The cantilever approaches the tip, makes contact, and applies compressive stress tothe interface. In these tests, we apply compressive forces of 1–5 µN. After the compressionphase, the cantilever is withdrawn from the pillar along a straight line at anangle θ to the cantilever surface (Figure 5.6). The angle θ varies from 0 ◦ to 90 ◦ toprovide loads varying between primarily normal and primarily shear. For high shearloads, the pillar is deflected and the side of the pillar contacts the substrate. We findthe forces present at the moment of failure by analyzing the force trace data (Figure5.7). The stresses at the interface increase until the interface breaks, at which pointthe measured forces either decrease rapidly or level off. Failure can be either a verticaldetachment from the surface or a slipping failure while the pillar is still in contact.A typical plot of the shear and normal force data can be seen in Figure 5.7. As inthe array testing, we look for failure events where the force vs. time plot undergoes anabrupt change in slope after the accumulation of force at the interface. These failurepoints are initially determined by looking at the maxima and minima of the normalforce data. We do not use the power method to determine the failure point. In thesetests, the stiffnesses of the force cantilever are comparable with the stiffnesses of the
CHAPTER 5. SINGLE PILLAR TESTING 53Figure 5.5: Profile image of single adhesive pillar and force cantilever. The mountingpin is visible on the left of the image. The texture on the pin is from shaping thepin to fit the PDMS sample. The block of PDMS is in the center of the photo witha single pillar protruding from the right side. The cantilever and die are in the lowerright of the photo.
CHAPTER 5. SINGLE PILLAR TESTING 54RelativeMotion+F normal+FlateralFigure 5.6: Diagram of mounted pillar and force-sensing cantilever. The black arrowsindicate the relative motion of the pillar and cantilever. The blue and green arrowsindicate the direction of positive forces exerted on the cantilever. This convention isused in the force plots.
CHAPTER 5. SINGLE PILLAR TESTING 55Figure 5.7: Single pillar force trace. This test is similar to the force traces performedin the previous chapter on adhesive arrays. The failure in this test is performed asa sliding test that will generate more shear than normal force. Notice that after theinitial failure that there is a reattachment event.
CHAPTER 5. SINGLE PILLAR TESTING 56adhesive pillar. Because of this condition, the velocity of the stage and the velocity ofthe substrate are different. In the case of the array measurements, the force plate wasmuch stiffer than the array and the velocity of the stage could be equated with therelative velocity of the adhesive backing and the substrate. We then examine thesepoints and if they appear incorrect, we manually determine the points by inspectingthe force traces for slope discontinuities using a graphical user interface coded inpython (Enthought Python Distribution, Enthought, Inc.). By using these points forall the different loading conditions, we create a limit curve.The normal and shear forces at these failure events are plotted as points in forcespace with normal force on the vertical axis and shear force on the horizontal axis.These force–time traces are collected for a variety of tension trajectories. The compiledforce time traces are analyzed to find the shear and normal forces at the releaseevent. We take the set of shear and normal forces at release and plot them. Whenthese points are plotted together, they create a limit curve  that separates forcepairs with stable attachment from force pairs that will detach.5.2 Data Collection and Analysis5.2.1 Piezo DriftAs the cantilever approaches the adhesive pillar, the normal force signal experiencesa significant drift. The adhesive pillar material, PDMS, is a dielectric material andwe expect uncontrolled static charge on the surface. Electrostatic attraction hasbeen ruled out as a possible cause since the sign of the drift remains the same whenthe cantilever is reversed. Figure 5.8 shows this signal drift when the cantileveris approached from the front as well as from the back. Although the signal of thecantilever being pushed and pulled is in the opposite direction, we see that the drift isin the same direction. This implies that the signal drift is not electrostatic attractiondeflecting the cantilever. Grounding the mounting pin did not improve the drift. Wedid not test to see if coating the sample in a conductive material would improve thedrift. Also, a pin without PDMS on the tip did not cause a signal drift. One possible
CHAPTER 5. SINGLE PILLAR TESTING 57Figure 5.8: Reversal Test of Cantilever. Cantilever was approached from front andback side of cantilever to determine if electrostatic attraction was the cause of thesignal drift.explanation is that the PDMS is affecting the implanted piezoresistors in a mannersimilar to the gate on a field-effect transistor. This drift is a well-behaved functionof the distance between the sample and the cantilever. To account for its effect, thevoltage immediately before contact is treated as the zero point and subtracted fromthe force voltage signal.5.3 ResultsThese limit curve tests give us two ways to look at the behavior of the adhesivepillars. The time-domain tests showing the force data allow us to see how the adhesivebehaves while in contact. We can see at what force the pillar fails and how the pillarbehaves during that failure. The force-domain limit curves allow us to determine
CHAPTER 5. SINGLE PILLAR TESTING 58what combinations of forces allow for stable adhesion. We will discuss each of thesebelow.5.3.1 Time Domain Force Trace ResultsThere is an interesting contrast in the adhesive behaviors of the array and the singleelement in these similar tests. In the array, we observe a sustained level of adhesionand shear while the adhesive is experiencing a sliding failure. The single terminalstructure sometimes displays large changes in adhesion during dragging which indicateevents of detachment and reattachment. This attachment and detachmentphenomenon is often called stick-slip. During the array sliding failure, the individualfibers of the array are losing contact and reattaching. Since there are thousands ofstructures this result is averaged out. This is another advantage afforded to fibrillaradhesive structures because of their distributed, redundant contacts. However,pronounced stick-slip was not seen in all force traces. When we use a more flexiblecantilever (629a03), we see pronounced stick-slip events more often. Though not idealfrom a measurement standpoint, the more flexible cantilever provides a more realistictesting of the adhesive pillar. This is because the pillar performs best when suspendedon a compliant structure to allow for conformation to the surface irregularities. Thisadhesive has been integrated with a compliant backing and showed improvement inits performance .The stick slip events with the more flexible cantilever can be seen in Figure 5.9.Notice that at the same time that the shear adhesion is lost due to the slip detachmentevent, there is also a loss in normal adhesion. When we use a stiffer cantilever (529b02)however, the amount of adhesion lost is less as we see in Figure 5.7. This could be areflection of the larger amount of deflection in the more compliant cantilever. Whenthe interface fails, the more compliant cantilever moves a larger distance and makesit more difficult to quickly reattach. The cantilever surfaces have not been wellcharacterized to determine if this is only due to the stiffness difference or is relatedto some irregularity on the surface of the cantilever.
CHAPTER 5. SINGLE PILLAR TESTING 59Normal Force (µN)Lateral Force (µN)3.02.52.01.51.00.50.0−0.5−1.0Normal Force (µN)Initial ContactInitial CompressionInterface Failure−1.50 1 2 3 4 5 6 7 8 93.02.52.01.51.00.50.0−0.5−1.0../024-20091124-sws10-ls/data/separated/p30 a02.pdfcantilever = 629a03sample = sws10Lateral Force (µN)Initial ContactInitial CompressionInterface Failure−1.50 1 2 3 4 5 6 7 8 9Time (sec)Figure 5.9: This force trace was performed using a more compliant cantilever than inFigure 5.7. Note that after the initial failure that there is a larger loss of force beforethe reattachment event.
CHAPTER 5. SINGLE PILLAR TESTING 60Shear Stress (kPa) Normal Stress (kPa)Predicted 2.7 11Measured 4.5 13Table 5.2: Comparison of extrapolated failure stress and observed failure stress foradhesive arrays. The single pillar measurement underestimates the force observed inthe array measurements.5.3.2 Single Wedge Limit CurveA single wedge limit curve is shown in Figure 5.10. This limit curve shows an interestingbehavior not seen in the array limit curves. For small shear loads, there is areduction in the amount of normal force capacity, consistent with pressure-sensitiveadhesive behavior. Once a threshold of approximately 2 µN of shear force is applied,the behavior changes to the frictional adhesion behavior. This low shear adhesivebehavior, in the context of an adhesive optimized for climbing, can be thought of asa parasitic adhesion. To overcome this parasitic force to detach would compromisethe efficiency and stability of an animal or robot using such an adhesive .do not observe this parasitic adhesion in the arrays. Unless the adhesive pillars failsimultaneously, we are unlikely to see this parasitic effect.The wedge limit surface shows that for near vertical pulloff directions, there isrelatively little change in the normal adhesive failure force observed. For near parallelpulloff directions, however, there is a clear dependence on preload, with largerpreload forces leading to improvement in both shear and normal forces at failure.This behavior is also observed in the adhesive setae of the tokay gecko .If we assume simultaneous attachment of all fibers with equal force, we can findthe predicted array adhesions byWeF s ρ s (5.1)were F s is the force per stalk predicted by the single pillar measurements and ρ s isthe density of stalks. For the corresponding arrays for this single structure the stalkdensity is 625 per mm 2 . Comparing the points on the limit curve with the highesttensile stress, and using 4.3 µN and 17 µN we generate the Table 5.2.
CHAPTER 5. SINGLE PILLAR TESTING 61Figure 5.10: Limit curve for single wedge element. Color denotes the angle of pulloff.The size of the plot elements represents the force at the maximum compressive load.
CHAPTER 5. SINGLE PILLAR TESTING 62In Table 5.2 we see that the measured normal force is greater than that predictedby the single pillar measurements. We believe that this discrepancy comes from thedifferent relative stiffnesses in the single pillar and array measurements. The arraymeasurement uses a force plate that is much stiffer than the array and can deformthe pillars more than is possible in the single pillar tests with the more compliantdual-axis cantilever.5.3.3 Non-Tapered Wedge Limit CurveIt is challenging to manufacture the tapered shape found in our adhesive pillars. Todetermine the effect of the tapered shape, isolated single adhesive pillars of uniformcross-section were fabricated and tested in the same way as the tapered to determinethe limit curve.The dimensions of the non-tapered pillar were chosen to match the height (60µm)and width (20µm) of the tapered pillar but with a range of thicknesses in the directionof bending. The thickness of the pillar tested (12µm) provides more lateral compliance(0.03 N/m) than the tapered pillar (0.15 N/m). This adjustment was to create a pillarsufficiently compliant to create side contact between the pillar and the force cantilever.A scanning electron microscope image of the nontapered and tapered pillars is shownin Figure 5.11The nontapered pillar limit curve is shown in Figure 5.12. The curve shows areduction of normal adhesive capacity with increasing shear force.In Figure 5.13, we see the limit curve of a tapered pillar and a non-tapered pillarshown on the same plot. These limit curves show that the tapered pillar exhibits agecko-like frictional adhesion behavior while the non-tapered pillar exhibits pressuresensitiveadhesive behavior.5.4 Slanted Beam Limit CurvesNatural fibrillar adhesive structures are usually at angle to the substrate less than90 degrees. We were curious about the performance of tapered structures that were
CHAPTER 5. SINGLE PILLAR TESTING 63Figure 5.11: SEM Images of pillar types. Both pillars share a base width of ∼20 µmand a height of ∼60 µm. The pillar in (a) is ∼20 µm thick at the base and tapers toa tip. The pillar in (b) is ∼12 µm thick at the base and has uniform thickness alongthe length of the beam.at an angle to the backing. However, fabrication issues of alignment between layersprevented us from creating tapered angled pillars. Using the degrees of freedomavailable in the test apparatus, we were able to vary the angle of the pillar withrespect to the force cantilever substrate. This variation of angle is depicted in Figure5.14. We conducted tests that varied the angle of the pillar in the plane defined bythe cantilever normal and the proximal-distal axis of the pillar.The data in Figure 5.15 show that as the angle between the substrate and thepillar is moved into the preferred direction (positive θ), the normal force capacity fora given amount of shear force increases. This corresponds to an increased stabilityfor an adhesive with a fixed shear load. The variation in normal force to break theinterface at zero shear load is much less than the variation at shear loads greater than2 µN. In this region, it seems likely that the adhesion is dictated by the shape of thetip rather than the compliance of the beam. The effect of the beam compliance onadhesion will be discussed in Chapter 6.
CHAPTER 5. SINGLE PILLAR TESTING 64Figure 5.12: Limit curve for single nontapered pillar element. Each plot point representsan adhesive failure. Notice the decline in normal force capacity with increasingshear force. The color depicts the angle of withdrawal of the cantilever. The size ofthe circle indicates the amount of compression applied before the tensile phase.
CHAPTER 5. SINGLE PILLAR TESTING 65Figure 5.13: Limit surfaces for tapered and non-tapered single pillars. Each datapoint reports the forces preceding a single failure event. Trials are run at 19 pullangles ranging between 0 degrees (vertical) and 90 degrees (shear). Each of theseangles is tested at two different levels of peak compressive load.
CHAPTER 5. SINGLE PILLAR TESTING 66Figure 5.14: Drawing of slant angle definition used in testing. Angle is between theback vertical face of the wedge structure and the normal to the cantilever surface.Positive angle is considered to be the preferred slant direction for the structure.
CHAPTER 5. SINGLE PILLAR TESTING 67Figure 5.15: Limit curves of single pillar at varying angles with respect to the forcecantilever surface. Each plot point represents an adhesive failure. The amount ofnormal adhesion force necessary for failure increases with the application of shearforce to the interface as the angle is moved from the anti-preferred to the preferredangle.Adhesive pillars that are inclined with respect to the substrate have a lower effectivestiffness. As the beam angle moves away from perpendicular, the load movesfrom axial to shear and the deflection is greater. This lower effective stiffness could beobserved as a function of the slant angle of the beam. Figure 5.16 shows the measuredrelation of the normal component of compliance with slant angle. This lower effective
CHAPTER 5. SINGLE PILLAR TESTING 68Figure 5.16: Plot of measured stiffness in the normal axis vs. the angle of the pillar.Highest stiffness is measured near zero degrees.modulus could improve the ability of the adhesive to engage with lower initial compressionforces. This would be advantageous for efficient and stable climbing sincethe initial compression forces must be balanced by the adhesion of the other contactsof a climbing animal or robot.These results point toward the importance of the leaning angle of the fibril in theperformance of the adhesive.
Chapter 6ModelingIn Chapter 5, different limit surfaces were observed depending on the shape of thebeam. The aim of this chapter will be to present models that can provide insight intothis behavior. We would like to develop a model that predicts these observed changesin the limit surface as a function of the beam shape. Such a model could allow forthe design of beams with engineered limit surfaces to provide the type of adhesiondesired for a specific application.Fibrillar adhesives are often modeled using contact models developed for hemisphericalcontacts . These models are applicable for low aspect ratio fibrils. Forhigh-aspect ratio fibrillar adhesives, models of adhesion incorporate the bending ofthe fibrils . These bending models use elastica beam theory  to predict theshape of the beam. To account for the highly anisotropic behavior of gecko adhesive,a model known as the ‘peel-zone’ model was proposed . This work attempts touse the ‘peel-zone’ model along the elastica beam model to predict the change in thelimit surface observed.6.1 Peel Zone ModelWe begin these modeling efforts with a description of the peel-zone model of fibrillaradhesion which attempts to capture gecko-like adhesive behavior. In the peel zonemodel, the central idea is that the area of the surface in contact gives rise to the69
CHAPTER 6. MODELING 70friction forces observed and the area in close proximity where the pillar is peelingaway from the substrate is responsible for the adhesion. The model assumes that theshear stress is uniform over the area in contact and that the resulting friction force isdirectly proportional to the amount of area in intimate contact. The adhesion forceis calculated by integrating the attractive force in the area in close proximity. Themodel finds that the adhesion force is an increasing function of the radius of curvatureof the beam in this area of close proximity or ‘peel zone’. An illustration of theseregions can be seen in Figure 6.1. The peel zone geometry applies to our situation inthat when the pillar is sufficiently sheared by the cantilever, the tip of the pillar isbent so that a length of the flat section of the pillar is in side contact (see Figure 6.12.The task is then to model the shape of the beam under the adhesion conditions ofour test, determine the size of the region in contact and the region in close proximityand then predict the forces the interface is capable of withstanding. This approachwill build on the peel-zone model, which lacks a consideration of the beam mechanicsof the fibril.6.2 Elastica ModelTo find the profile of the beam for use in the peel-zone predictions of adhesive force,we use the elastica beam model. The elastica beam model  allows the calculationof a beam profile for large angle deflection of an elastic beam. The elastica model ofbeam deflection has been used by researchers in the calculation of the deflection ofmicrofabricated polymer structures [40, 43]. The elastica model is used because themore familiar model, the Euler beam model, is not valid for large angle deflections.Unlike the Euler beam model, the elastica model does not rely on an approximationof the curvature. This model of beam deformation will allow us to simulate the beamprofile under loading. To solve for the beam profile given a load and shape, we solvethe equationM = κEI (6.1)
CHAPTER 6. MODELING 71Contact AreaPeel ZoneFigure 6.1: Pillar peel diagram. The peel zone model assumes uniform shear stressdistributed over the contact area. The peel zone is defined as the region with contactclose enough for significant van der Waals force. The total force transmitted alongthe beam is the vector sum of the shear force in the contract area and normal forcein the peel zone area.where M is the bending moment on the beam, E is the elastic modulus of thematerial, I is the moment of area of the beam, and κ is the curvature of the beam.
CHAPTER 6. MODELING 72In cartesian coordinates, the curvature κ is expressed exactly asκ =y ′′. (6.2)(1 + y ′2 )3/2Euler beam theory assumes that the slope (y ′ ) is negligible compared to unity andthat the curvature (κ) can be approximated by the second derivative (y ′′ ). Instead ofcartesian coordinates, the beam is expressed with parameterized coordinates of arclength (s) and tangent angle along the beam (ψ(s)), reminiscent of the Frenet-Serretformulas. These coordinates allow the curvature to be expressed exactly asκ = dψds . (6.3)This elastica formulation allows us to sidestep the small angle deflection restrictionsof Euler beam theory.The other benefit of expressing the beam slope as aposition of arc length is that the beam shapes observed in experiments that wouldbe multivalued functions in cartesian coordinates, are expressed easily. The model aspresented here does not take into account shear strain in the beam, which can affectthe results.Using this alternate set of coordinates, the beam equation (Eq. (6.1)) becomesM = κEI = dψ EI, (6.4)dsIn general, M and I are functions of the arc length, s, and we have the first-orderdifferential equationdψds = M(s)EI(s) . (6.5)This function can be solved either analytically or numerically depending on theform of the resulting functions for the load and shape of the beam. We now turnto a discussion of the loads and beam shapes in our adhesive wedge structures. Weapproximate the loading with a combination of point loads and moments to reflectthe shape observed during testing.
CHAPTER 6. MODELING 73Figure 6.2: Elastica coordinates for point load. x and y denote the cartesian systemused to describe beam displacement. s is the displacement along the beam, and ψ isthe angle of the beam with respect to the x-axis at the point s. P is the load, r isthe lever arm for the moment at point s along the beam. The small triangle showsthe decomposition of ds along the x and y axes.6.2.1 Cantilever with Point Load at EndConsider the case of a point load applied at the end of a cantilevered beam. Followingthe treatment in  we apply this point load to an elastica beam representing theadhesive pillar. In Figure 6.2 we have the geometry of our horizontal cantilever withthis point load. To solve the bending equationdψds = M(s)EI(s) . (6.6)we must find the bending moment (M) and the moment of the beam (I) in termsof the variables s and ψ.
CHAPTER 6. MODELING 74To find the bending moment along the beam, we look at the vector productbetween the displacement vector and the applied load. The magnitude of the momentis equal to the magnitude of the cross product between the vector from the point onthe beam to the load (r(s)) and the load (P ).M = r(s) × P (6.7)If we decompose the load, P , into shear and axial components and project thedisplacement vector r(s) onto the x and y axes, (see Figure 6.2) we can express themagnitude of the moment asM = P y r x − P x r y . (6.8)If we substitute this expression for the moment into equation (6.6) we obtaindψds EI = P yr x − P x r y (6.9)By differentiating the equation with respect to s, the components of the displacementvector ⃗r become trigonometric functions of ψ, which allows us to express theequation purely in terms of ψ. Note thatr x (s) =∫ Lscos ψ ds = −∫ sDifferentiating this expression by the arc length, we findLcos ψ ds (6.10)Similarly, we find thatdr x (s)s= − d ds∫ Lscos ψ ds = − cos ψ. (6.11)dr y (s)s= sin ψ. (6.12)By substituting Eqs.(6.11) and (6.12) into Eq. (6.9), we obtaind 2 ψds 2 EI = −P y cos ψ + P x sin ψ. (6.13)
CHAPTER 6. MODELING 75This equation is solved numerically to determine the beam shape for a given pointload. This second-order equation is reduced to two coupled first-order equations forthe numerical calculation.Equation (6.13) holds for a beam of uniform cross-section.The beams underconsideration have a wedge shape. These beams are modeled as a truncated prism asshown in Figure 6.3. To express the taper, there are two length scales for the pillar.The first is the actual length, the second is the distance from the base where theplanes defined by the sides of the pillar would intersect. The thickness of the beamis then a linear function of the arc length variable s.b(s) =b 0(1 − 1L T)s (6.14)The moment of area of the beam includes this term for the thicknessI(s) = 1 wb(s) 3(6.15)12 L 3In the case of a non-uniform cross-section of the beam, the derivatives of themoment of inertia of the beam with respect to the arc length are non-zero. In thiscase, the equation isdI dψds ds + ψI(s)d2 ds 2=(P x sin ψ − P y cos ψ) 1 Edxds[d 2 ψds = (P 2 x sin ψ − P y cos ψ) 1 E − dI ]dψ 1ds ds I(s)(6.16)(6.17)Once the slope has been determined as a function of the arc length, the cartesiancoordinates of the beam position can be determined by integrating the slope function.For the point load, the boundary conditions are the undeflected slope at the baseof the beamψ| s=0 = 0 (6.18)
CHAPTER 6. MODELING 76Figure 6.3: Dimensions used in the simulation of the tapered beam. The length l isthe physical extent of the beam while the taper length l t is the point at which thebeam thickness would vanish. Due to imperfections in the fabrication process, theselengths are not the same. s is the arc length along the beam and b and t are thedimensions at the base of the structure. The tapered structures tested in this workhave dimensions approximately l = 50 µm, b,t = 20 µm, and l t =80 µm.
CHAPTER 6. MODELING 77and the zero curvature at the end of the beamψ ′ | s=L =0. (6.19)6.2.2 Fixed Slope at End of BeamThe actual loading condition of the beam during testing applies a shear load butgenerally provides an additional constraint that the end of the beam is parallel to thesubstrate (ψ = π/2).In this case, the boundary conditions are the slopes at both ends of the beamψ| s=0 = 0 (6.20)ψ| s=L = π 2(6.21)In this case, the curvature at the end of the beam is a free parameter. This is incontrast with the point load case where the curvature is zero at the end. A shootingmethod solution is used since neither of these cases provides an initial condition thatcan be used to uniquely solve the beam. The initial curvature (ψ| s=0 ) is guessed andthe solution is performed until the condition at the end of the beam matches theboundary condition.6.3 Numerical Results6.3.1 ValidationWe solve the differential equation governing the beam shape (Equation (6.17)) numerically.Before using the model to simulate beam deformations, we pause to performsome simple verifications. We verify the model for small point loads by comparingit to the Euler model of beam bending for a point load. Figure 6.5 shows a plot ofthe tip displacement as a function of the load. The models are in good agreement for
CHAPTER 6. MODELING 78Figure 6.4: Depiction of parameters used in side contact elastica model. The load Pis proportional to l, the length in contact. The point moment M is applied at thepoint where the pillar begins to peel out of contact.
CHAPTER 6. MODELING 79Figure 6.5: Normalized tip deflection as a function of load for both the Euler beammodel and the elastica numerical model. The models have good agreement for smallerloads and diverge with the application of larger loads. This plot is for the typicalpillar dimensions and the normalized loads correspond to approximately 0-4µN.small loads. We expect the models to diverge for larger loads where the beam slopeis no longer negligible.The next demonstration of the model is the beam profile under various loadingconditions. The first of these loading conditions is that of a point shear load. Figure6.6 shows a simulated pillar under increasing shear load. The beam shows increaseddeflection with increased shear load. The profile however, does not match the profileobserved in the testing. A point load does not result in the end of the beam bendingover to be perpendicular to the base of the beam. To get profiles that match thetesting of the adhesive pillars, we add a point moment condition.
CHAPTER 6. MODELING 80Figure 6.6: Profile predicted by elastica model of various beam loadings. Note thatthe beam does not become vertical in these cases. Under experimental conditions thebeam is bent over at the same shear force load. For this reason, we impose the extrapoint moment condition to get a more realistic profile in the model.
CHAPTER 6. MODELING 81Figure 6.7: Constrained end angle with varying point shear load. Model simulatesa tapered beam of nominal dimensions and constrains the end angle to be 90 ◦ . Themagnitude of the shear load is varied and the beam profile is plotted.Figure 6.7 is a plot of a simulation of an adhesive pillar constrained so that the endangle is 90 degrees from the base of the pillar. The pillar also has increasing amountsof normal shear load applied. If we compare this profile to the images observedexperimentally (Figure 6.12), the simulation seems more plausible than those givenfor only a point moment.It is difficult to accurately compare the profiles for a given shear force applied. Theimage quality of the microscope system made accurate measurement of the profile andlength of side contact difficult. Another compounding factor is that the piezoresistiveforce sensors are light-sensitive. This invalidates the calibration curves, which areobtained under dark conditions.
CHAPTER 6. MODELING 826.3.2 Limit Surface SimulationWith the model giving plausible results, we start to simulate the behavior of uniformand tapered beams looking for differences in the behavior that may explain the limitcurve differences we observe. We start by looking at the profiles of the beams underthe experimental loading conditions. We then simulate the loading of the beam inthe experiment and observe the beam geometry. By extracting the beam geometry inthe regions of interest in the peel-zone model, we hope to gain insight into the limitcurve.When we plot the profiles of these two pillars for the condition of having the endangle of the beam at 90 degrees we see a clear qualitative difference in their profiles.Figure 6.8 shows two beams of dimension 60µm long with 20µm by 20µm bases. Thedifference is that the tapered beam would converge to a point at 80µm, giving a 5µmthick tip, which is reasonable in our fabricated structures. The plot shows that forthe uniform thickness pillar that the radius of curvature is constant over the lengthof the beam. In the absence of a point load, the beam is indeed a circular arc. Thetapered beam however, shows that the curvature is concentrated at the end of thebeam. In the absence of a point load, the bending moment is uniform over the beambut the non-uniform moment of inertia leads to a non-uniform curvature.In the previous chapter we showed the difference in the observed limit curve dependingon the shape of the pillar. For frictional adhesion to occur, the peel-zonesuggests that as the area in contact increases, the radius of the beam in the peelzone increases. As the radius of curvature increases, the normal force capacity of thefibril increases, giving a frictional adhesion limit curve. In contrast, the limit curveobserved in pressure-sensitive adhesives would be observed if the radius of curvaturein the peel-zone decreased as the length in contact increased.Glassmaker and Hui  show that for a beam in a similar geometry that the radiusof curvature in this peel zone is an increasing function of the moment of inertia ofthe beam. Due to the taper, the thickness and moment of inertia of the pillar at thepeel-zone increases and the radius of curvature at the point of peeling increases. Asthis radius increases, the length of the zone close enough for attractive force increases,allowing for more normal adhesion and the adhesive demonstrates frictional adhesion.
CHAPTER 6. MODELING 83Figure 6.8: Comparison between beam profile for a uniform beam and a taperedbeam with the end at 90 degrees. Beam profile is simulated using the elastica model.The curvature for the uniform beam is constant throughout the beam while for thenon-uniform beam it is concentrated at the end of the beam.
CHAPTER 6. MODELING 84Figure 6.9: Radius of curvature at peel-zone as a function of the length of fibril incontact for a tapered beam. The radius of curvature adjacent to the length of thebeam in contact is calculated at varying lengths of beam in side contact at 90 ◦ . Noshear for was applied in this simulation.In contrast, the non-tapered beam has a uniform moment of inertia and does not showthe increase in normal force with increasing shear force.This section will show simulations that suggest that for a tapered and non-taperedbeam this is the predicted behavior. Our strategy is then to observe the changes inthis radius of curvature as we hold an increasing fraction of the beam in contact, aswould be necessary to sustain increasing shear or friction force.Using the dimensions appropriate for the structures under test we simulate thebeam profile.If we approximate the shear adhesion by the cylindrical JKR approximation and ignore the tip radius and its effect on the adhesion at low shear values, we can
CHAPTER 6. MODELING 85Figure 6.10: Radius of curvature at peel-zone as a function of the length of fibril incontact for a non-tapered beam. The radius of curvature adjacent to the length ofthe beam in contact is calculated at varying lengths of beam in side contact at 90 ◦ .No shear for was applied in this simulation.
CHAPTER 6. MODELING 86simulate the limit curve. The simulation shown in Figure 6.11, that as the shearadhesion increases, for a 20µm tip (no taper), that there is an decrease in the normaladhesion capacity. For smaller tip thicknesses, this situation reverses, with the limitcurve showing negative slope for 2 and 5 µm tips. It is interesting to note that for anintermediate tip thickness there is a curve with near-zero slope.These results suggest that by tailoring the pillar shape such that the local radiusof curvature at the point of contact is an increasing function of shear load, frictionaladhesion can be achieved. While the geometries are very different, the tokay geckoadhesive behaves in a similar fashion. The initial contact of the gecko adhesive iswith the flat edges of the spatulae. With shear loading, the spatulae are bent intoflat contact resulting in a large increase in shear adhesion. We must be cautious inusing this beam model to explain gecko adhesion but we do observe similarities inthese very simple tapered structures.
CHAPTER 6. MODELING 87Figure 6.11: Limit curve simulation. Simulation computes the normal pull-off forceusing the cylindrical JKR formula for an elastica beam with a shear force and correspondinglength in contact. The different curves depict a spectrum between taperedand uniform beams. The 20 µm tip is a uniform pillar and the 2 µm tip has thehighest degree of taper.
CHAPTER 6. MODELING 88Figure 6.12: Photo of single wedge in cantilever test setup under deflection. Thecantilever is the small vertical stripe in the center of the photo. The normal forceaxis is horizontal and the shear force axis is in the vertical direction.
Chapter 7Conclusion7.1 SummaryInspired by the unique frictional adhesion property of the gecko’s adhesive, we fabricateda microstructured adhesive with tapered pillars. Testing of arrays of theseadhesive pillars revealed that the adhesive displayed the frictional adhesion property.This means that the adhesive becomes more tenacious in response to loading. Specifically,that the amount of holding capacity normal to the surface increases as theamount of shear stress at the interface is increased.To determine if this frictional adhesion property is due to the fibril or due to thearray, we tested a single adhesive fibril using a sensitive dual-axis micromachinedcantilever. Using this cantilever we determined that the adhesive behavior of thesingle pillar differs from the array. First, the single pillar shows randomly occurringfailures that are averaged out in the arrays. Second, the single pillar shows a limitcurve whose behavior at low values of shear stress differs from the array’s limit curve.The single pillar shows a normal force adhesion at low shear values that is not evidentin the limit curve of the array.We varied the pillar shape to determine if the tapered pillar shape contributes tothe frictional adhesion behavior. To test, we fabricated adhesive pillars of uniformcross section that lacked the tapered shape. These structures did not exhibit frictionaladhesion and instead displayed the type of adhesion found in pressure-sensitive89
CHAPTER 7. CONCLUSION 90adhesives. We also varied the angle that the pillar made with the cantilever surfaceto investigate the effect of leaning angle. The limit curve showed an enhancement ofthe ratio of normal force to shear force with leaning angle.Last, we presented modeling of these adhesive cantilevers predicting the differencesin adhesion behavior of tapered and nontapered pillars. The modeling also predictedthe enhancement of the adhesion as the leaning angle increased.The results presented here will help inform the design of fibrillar elements that arecustomized for the application. Frictional adhesion, a property useful for climbing applicationscan be achieved using tapered, slanted beams. Nontapered beams, however,may be optimal for applications where frequent reattachment and easy detachmentare not important.7.2 Future WorkThis thesis presents work important for synthetic fibrillar adhesives. The fabricationtechniques in this work are difficult, labor intensive, and often low yield. The developmentof more robust and repeatable manufacturing methods make fabricationeasier and aid in development of improved adhesives. If a more robust mold could bemade, then large scale manufacturing of these fibrillar adhesives becomes possible.Another opportunity for improvement is in the modeling of the behavior of thesefibrillar elements. It would be very useful to validate the model using careful imagingof pillars under load. Finite Element Models using distributed rather than lumpedforces would also increase confidence in the results presented here.Improvements in these areas could enable adhesive technologies that in additionto the ability to adhere, have the ability to disengage quickly and cleanly. Theseadhesives can improve the capabilities of climbing robots or the throughput of flatpanel manufacturing and could eventually find a place in consumer adhesives.
Appendix ABeam Compliance CharacterizationIn addition to the limit curve testing of the cantilever, we have tested the complianceof the pillar. Testing of the compliance was used to help validate simulations of thebeam profile in the previous chapter. This appendix describes the testing of thecompliance of PDMS adhesive pillars in the normal and shear directions.A.1 ComplianceA.1.1Axial ComplianceNormal compliance was measured by bringing the flat end of the dual-axis cantileverinto contact with the top of the microwedge tip. The cantilever was then moved alongthe axial dimension of the adhesive pillar to put the pillar into axial compression. Thedeflection of the pillar can be inferred as well as the force applied, yielding a springconstant for the adhesive pillar. The system is essentially two springs in parallel, onespring is the dual-axis cantilever spring in the normal direction, the other spring is theadhesive pillar. This effective spring constant is the force measured by the cantileverdivided by the displacement of the stage. The slope of the curve in figure A.1 is thiseffective spring constant of the system. Defining k E as the effective spring constant,k P as the pillar spring constant and k C as the cantilever spring constant, the relation91
Normal Microwedge Force vs. CompressionCantilever 529b02 − Sample SWS720000127−sws7−ncAPPENDIX A. BEAM COMPLIANCE CHARACTERIZATION 92Preload Force (µN)108642k=5.0k=2.0k=1.000 1 2 3 4Measured Compression (µm)Figure A.1: Axial compression for tapered adhesive pillar. Sample was rotated aboutlong axis. The spread in the data illustrates the uncertainty arising from placementalong the tip of the force cantilever.between them is1= 1 − 1k P k E k C(A.1)We measure the k E of the system and then use the known spring constant of thecantilever k C to calculate the pillar’s spring constant. The tapered pillar is predictedto be about 2–3 times stiffer than the cantilever’s normal compliance. In this case,the correction for the spring constant is necessary for a meaningful measurement.Figure A.1 shows measured data of a tapered adhesive pillar sample under axialcompression. The measured compression axis is the compression of the pillar. Theplot has data from four rotation angles. Because of the variability in normal force asa function of placement on the tip of the cantilever, there is a large range of measuredspring constants.
APPENDIX A. BEAM COMPLIANCE CHARACTERIZATION 93The modeled spring constant for a tapered beam is given byk = Ewb a − 1L log a .(A.2)For numbers matching the tapered pillar structure (E modulus of 1MPa w andb the base and width of the structure are 20 µm, L = 60 µm and a =0.25. Here arepresents the amount of taper in the pillar, with a = 1 being a uniform beam, andwith a = 0 describing a perfect point. The resulting spring constant is k =3.6 N/mwhich is in within the spread shown in A.1.A.1.2Lateral ComplianceThe lateral compliance measurement is similar to the normal measurement but insteadused the side of the cantilever and pressed in the lateral direction. Two differencesarise in this case. The first is that the sensitivity to the point of contact is reducedwhen using the cantilever in the shear direction. This is because the cantilever usesa truss structure. The second difference is that the cantilever has a different springconstant in the lateral direction. Because the compliance of the pillar is much greaterin shear than axial, the force cantilever is stiffer than the structure under test. Itwas the opposite in the axial compliance measurement. Despite the relative springconstants, the correction described above was also performed on these measurements.These values are clustered around k =0.1 N/m. Using the elastica model describedin Chapter 6 and the values used above in the axial compression, we obtain aspring constant of 0.08 N/m. This value is in excellent agreement with the measuredvalue.
APPENDIX A. BEAM COMPLIANCE CHARACTERIZATION 94Shear Microwedge Force vs. Microwedge DeflectionCantilever 529b02 − Sample SWS620081113−1−sb3Preload Force (µN)21k=0.20k=0.10k=0.0500 5 10 15Measured Compression (µm)Figure A.2: Lateral compliance for tapered adhesive pillar. The measured compressionis in the lateral direction.
Bibliography C. Gay and L. Leibler, “Theory of tackiness,” Physical Review Letters, Jan 1999. A. Peattie, C. S. Majidi, A. Corder, and R. J. Full, “Ancestrally high elasticmodulus of gecko setal -keratin,” Journal of The Royal Society Interface, vol. 4,no. 17, pp. 1071–1076, Jan 2007. J. Israelachvili, Intermolecular & Surface Forces. Academic Press, 1985. C. Thornton, “Interparticle sliding in the presence of adhesion,” J. Phys. D:Appl. Phys, vol. 24, pp. 1942–1946, Oct 1991. H. Yoshizawa, Y.-L. Chen, and J. Israelachvili, “Fundamental mechanisms ofinterfacial friction. 1. relation between adhesion and friction,” J. Phys. Chem.,vol. 97, pp. 4128–4140, Jun 1993. A. Savkoor and G. Briggs, “The effect of tangential force on the contact ofelastic solids in adhesion,” Proceedings of the Royal Society of London. Series A,Mathematical and Physical Sciences (1934-1990), vol. 356, no. 1684, pp. 103–114,1977. H. Hertz, “Uber die beruhrung fester elasticher korper,” Journal fur die reineund angewandte mathematik, vol. 92, pp. 156–171, May 1881. K. Johnson, K. Kendall, and A. Roberts, “Surface energy and the contact ofelastic solids,” Proceedings of the Royal Society of London. Series A, Jan 1971.95
BIBLIOGRAPHY 96 K. Autumn, A. Dittmore, D. Santos, M. Spenko, and M. R. Cutkosky, “Frictionaladhesion: a new angle on gecko attachment,” Journal of Experimental Biology,vol. 209, pp. 3569–3579, Jan 2006. K. Autumn, S. Hsieh, D. Dudek, J. Chen, C. Chitaphan, and R. J. Full, “Dynamicsof geckos running vertically,” Journal of Experimental Biology, vol. 209,pp. 260–272, Jan 2006. A. Geim, S. Dubonos, I. Grigorieva, K. Novoselov, A. Zhukov, and S. Y. Shapoval,“Microfabricated adhesive mimicking gecko foot-hair,” Nature Materials,vol. 2, pp. 461–463, Jan 2003. S. Gorb, M. Varenberg, A. Peressadko, and J. Tuma, “Biomimetic mushroomshapedfibrillar adhesive microstructure,” Journal of The Royal Society Interface,vol. 4, pp. 271–275, Jan 2007. L. Ge, S. Sethi, L. Ci, P. Ajayan, and A. Dhinojwala, “Carbon nanotube-basedsynthetic gecko tapes,” Proceedings of the National Academy of Sciences, vol.104, no. 26, pp. 10 792–10 795, Jan 2007. B. Schubert, J. Lee, C. S. Majidi, and R. S. Fearing, “Sliding-induced adhesion ofstiff polymer microfibre arrays. ii. microscale behaviour,” Journal of The RoyalSociety Interface, Jan 2008. M. P. Murphy, B. Aksak, and M. Sitti, “Adhesion and anisotropic friction enhancementsof angled heterogeneous micro-fiber arrays with spherical and spatulatips,” J. Adhesion Sci. Technol, vol. 21, no. 12-13, pp. 1281–1296, Jan 2007. S. Kim and M. Sitti, “Biologically inspired polymer microfibers with spatulatetips as repeatable fibrillar adhesives,” Applied Physics Letters, vol. 89, no. 26, p.261911, Jan 2006. L. Qu, L. Dai, M. Stone, Z. Xia, and Z. L. Wang, “Carbon nanotube arrays withstrong shear binding-on and easy normal lifting-off,” Science, vol. 322, no. 5899,pp. 238–242, Oct 2008.
BIBLIOGRAPHY 97 B. Aksak, M. Sitti, A. Cassell, J. Li, and M. Meyyappan, “Friction of partiallyembedded vertically aligned carbon nanofibers inside elastomers,” AppliedPhysics Letters, Jan 2007. J. Lee, R. S. Fearing, and K. Komvopoulos, “Directional adhesion of geckoinspiredangled microfiber arrays,” Applied Physics Letters, vol. 93, no. 19, p.191910, Jan 2008. E. Arzt, S. Gorb, and R. Spolenak, “From micro to nano contacts in biologicalattachment devices,” Proceedings of the National Academy of Sciences of the . . . ,vol. 100, no. 19, pp. 10 603–10 606, Jan 2003. A. del Campo, C. Greiner, and E. Arzt, “Contact shape controls adhesion ofbioinspired fibrillar surfaces,” Langmuir, vol. 23, no. 20, pp. 10 235–10 243, Jan2007. B. Aksak, M. P. Murphy, and M. Sitti, “Adhesion of biologically inspired verticaland angled polymer microfiber arrays,” Langmuir, vol. 23, pp. 3322–3332, Jan2007. H. Jeong, J. Lee, H. Kim, S. Moon, and K. Suh, “A nontransferring dry adhesivewith hierarchical polymer nanohairs,” Proceedings of the National Academy ofSciences, Jan 2009. D. Santos, M. Spenko, A. Parness, S. Kim, and M. R. Cutkosky, “Directionaladhesion for climbing: theoretical and practical considerations,” Journal of AdhesionScience and Technology, vol. 21, no. 12-13, pp. 1317–1341, 2007. N. Rizzo, K. Gardner, D. Walls, N. Keiper-Hrynko, T. Ganzke, and D. Hallahan,“Characterization of the structure and composition of gecko adhesive setae,”Journal of The Royal Society Interface, vol. 3, no. 8, pp. 441–451, 2005. R. Ruibal and V. Ernst, “The structure of the digital setae of lizards,” Journalof Morphology, vol. 117, no. 3, 1965.
BIBLIOGRAPHY 98 K.-Y. Hung, H.-T. Hu, and F.-G. Tseng, “Application of 3d glycerolcompensatedinclined-exposure technology to an integrated optical pick-uphead,” J. Micromech. Microeng., vol. 14, no. 7, pp. 975–983, 2004. H. Sato, Y. Houshi, and S. Shoji, “Three-dimensional micro-structures consistingof high aspect ratio inclined micro-pillars fabricated . . . ,” Microsystem Technologies,vol. 10, pp. 440–443, Jan 2004. M. Han, “3d microfabrication with inclined/rotated uv lithography,” Sensorsand Actuators A: Physical, vol. 111, no. 1, pp. 14–20, 2004. Y.-K. Yoon, J.-H. Park, and M. G. Allen, “Multidirectional uv lithography forcomplex 3-d mems structures,” J Microelectromech S, vol. 15, no. 5, pp. 1121–1130, 2006. M. Sitti and R. S. Fearing, “Synthetic gecko foot-hair micro/nano-structures asdry adhesives,” Journal of Adhesion Science and Technology, vol. 17, Jan 2003. D. Santos, “Contact modeling and directional adhesion for climbing robots,”Ph.D. dissertation, Stanford University, Oct 2007. A. Parness, D. R. Soto, N. Esparza, N. Gravish, M. Wilkinson, K. Autumn, andM. R. Cutkosky, “A microfabricated wedge-shaped adhesive array displayinggecko-like dynamic adhesion, directionality and long lifetime,” Journal of theRoyal Society, vol. 6, no. 41, pp. 1223–1232, Jan 2009. A. Parness, “Micro-structured adhesives for climbing applications,” Ph.D. dissertation,Stanford University, Feb 2010. B. Chui, T. Kenny, H. Mamin, B. Terris, and D. Rugar, “Independent detectionof vertical and lateral forces with a sidewall-implanted dual-axis piezoresistivecantilever,” Applied Physics Letters, vol. 72, no. 11, pp. 1388–1390, Jan 1998. K. Autumn, Y. Liang, S. Hsieh, W. Zesch, W. Chan, T. Kenny, R. S. Fearing,and R. J. Full, “Adhesive force of a single gecko foot-hair.” Nature, vol. 405, no.6787, pp. 681–685, Jan 2000.
BIBLIOGRAPHY 99 G. Hill, “Dual-axis mems force sensors for gecko adhesion studies,” Ph.D. dissertation,Stanford University, Feb 2009. S. Goyal, A. Ruina, and J. Papadopoulos, “Planar sliding with dry friction part1. limit surface and moment function,” Wear, vol. 143, pp. 307–330, 1991. A. Asbeck, S. Dastoor, A. Parness, L. Fullerton, N. Esparza, D. R. Soto,B. Heyneman, and M. R. Cutkosky, “Climbing rough vertical surfaces with hierarchicaldirectional adhesion,” IEEE International Conference on Robotics andAutomation, 2009. C. S. Majidi, R. E. Groff, and R. S. Fearing, “Attachment of fiber array adhesivethrough side contact,” Journal of Applied Physics, vol. 98, no. 10, p. 103521, Jan2005. R. Frisch-Fay, Flexible Bars. Butterworth and Co., 1962. Y. Tian, N. Pesika, H. Zeng, K. Rosenberg, and B. Zhao, “Adhesion and frictionin gecko toe attachment and detachment,” Proceedings of the National Academyof Sciences, vol. 103, no. 51, pp. 19 320–19 325, Jan 2006. Y. Xiang and D. A. Lavan, “Analysis of soft cantilevers as force transducers,”Applied Physics Letters, vol. 90, no. 13, p. 133901, Jan 2007. N. Glassmaker and C.-Y. Hui, “Elastica solution for a nanotube formed by selfadhesionof a folded thin film,” Journal of Applied Physics, vol. 96, no. 6, pp.1–6, Aug 2004. J.-J. Wu, “Adhesive contact between a cylinder and a half-space,” J. Phys. D:Appl. Phys, vol. 42, p. 155302, Jul 2009.